Optically pumped 1.3 μm room-temperature InAs quantum-dot ... · PDF file Optically pumped...
Embed Size (px)
Transcript of Optically pumped 1.3 μm room-temperature InAs quantum-dot ... · PDF file Optically pumped...
Optically pumped 1.3 μm room-temperature InAs quantum-dot micro-disk lasers directly grown on (001) silicon YATING WAN,1,† QIANG LI,1,† ALAN Y. LIU,2,† ARTHUR C. GOSSARD,2,3 JOHN E. BOWERS,2,3
EVELYN L. HU,4 AND KEI MAY LAU1,* 1Department of Electronic and Computer Engineering, Hong Kong University of Science and Technology, Clear Water Bay, Kowloon, Hong Kong, China 2Materials Department, University of California, Santa Barbara, California 93106, USA 3Department of Electrical and Computer Engineering, University of California, Santa Barbara, California 93106, USA 4School of Engineering and Applied Sciences, Harvard University, Cambridge, Massachusetts 02138, USA *Corresponding author: [email protected]
Received 16 February 2016; revised 8 March 2016; accepted 9 March 2016; posted 10 March 2016 (Doc. ID 259455); published 1 April 2016
Direct integration of high-performance laser diodes on silicon will dramatically transform the world of photonics, expedit- ing the progress toward low-cost and compact photonic integrated circuits (PICs) on the mainstream silicon platform. Here, we report, to the best of our knowledge, the first 1.3 μm room-temperature continuous-wave InAs quantum- dot micro-disk lasers epitaxially grown on industrial- compatible Si (001) substrates without offcut. The lasing threshold is as low as hundreds of microwatts, similar to the thresholds of identical lasers grown on a GaAs substrate. The heteroepitaxial structure employed here does not require the use of an absorptive germanium buffer and/or dislocation filter layers, both of which impede the efficient coupling of light from the laser active regions to silicon waveguides. This allows for full compatibility with the extensive silicon-on- insulator (SOI) technology. The large-area virtual GaAs (on Si) substrates can be directly adopted in various mature in-plane laser configurations, both optically and electrically. Thus, this demonstration represents a major advancement toward the commercial success of fully integrated silicon photonics. © 2016 Optical Society of America
OCIS codes: (140.5960) Semiconductor lasers; (140.3948)
Microcavity devices; (230.5590) Quantum-well, -wire and -dot
Optical interconnects have been playing an increasingly impor- tant role in high-performance silicon electronics, while high- dissipation electrical-interconnects pose a major roadblock to efficient operation and higher bandwidths [1–4]. To best leverage the economies of scale of silicon, development of com- plementary metal-oxide-semiconductor (CMOS)-compatible optical components is of paramount importance [5–7]. Mono- lithic growth of III–V photonic materials on silicon provides
the best route toward low-cost and scalable integration, pro- vided crystal defects associated with material incompatibility can be sufficiently reduced . Of the suite of optical compo- nents, highly efficient long-wavelength lasers are the most sensitive monitors of the quality of III–V/silicon hetero- integration . Quantum dot (QD) active layers grown on lattice-matched substrates have already shown their capability for lasers with low-threshold densities and temperature- independent operation [9,10]. In addition, the reduced sensi- tivity of QDs to defects and their unique capability of filtering dislocations make them an ideal candidate for the active layers of hetero-integrated III–V on Si optical sources [11,12]. In this Letter, we utilized InAs QDs monolithically grown on pre- patterned on-axis (001) Si substrates to achieve room-temper- ature continuous-wave (CW) lasing in a micro-disk resonator. The micro-disk cavities allow for rapid feedback of the QD performance and promote high-quality factor and dense inte- gration for short-reach communication links . The emis- sion is in the 1.3 μm telecommunication band, with low thresholds down to a few hundreds of microwatts. Thus, the InAs QD micro-disk lasers fabricated on Si (001) substrates without intervention of thick and absorptive buffer layers hold high promise for cost-effective integration of low-threshold optical sources on Si.
There has been much recent progress for InAs/GaAs quan- tum dot (QD) lasers monolithically grown on Ge or Ge-on-Si substrates [14–19], where intermediate buffer layers are used to reduce the number of dislocations and their intrusion into the active layer of the laser. These intermediate buffers, typically germanium and subsequent dislocation filter layers, are absorp- tive and relatively thick. Such layers limit efficient coupling from the active laser regions to silicon waveguides and preclude potential incorporation in the extensive SOI technology well developed in silicon photonics . Furthermore, the require- ment of using few-degree offcut Si substrates for antiphase domain (APD) suppression inevitably compromises its full
1664 Vol. 41, No. 7 / April 1 2016 / Optics Letters Letter
0146-9592/16/071664-04 Journal © 2016 Optical Society of America
compatibility with the prevailing Si CMOS manufacturing processes.
To bypass the need for the absorptive buffer layers and offcut Si substrates, we have recently demonstrated highly or- dered, regular arrays of planar GaAs nanowires on industrial- standard (001) silicon by combining the epitaxial necking effect with a design of diamond-shaped Si pockets . Coalescence of these planar nanowires led to high-quality, antiphase- domain-free GaAs-on-V-grooved-Si (GoVS) templates. On the GoVS templates, InAs QDs showed superior structural and optical properties over those grown on conventional offcut Si substrates . Therefore, the GoVS template forms the initial platform of our devices. We grew the GoVS template with 1 μm GaAs coalesced thin film in an Aixtron AIX- 200/4 metal-organic chemical vapor deposition (MOCVD) system, using the same procedure [Fig. 1(a)], as detailed in . A root-mean-square roughness of ∼2 nm across a scan- ning area of 5 μm × 5 μm on the as-grown GoVS template was obtained by atomic force microscopy (AFM) measurements [Fig. 1(b)]. The coalesced thin films are so flat that additional chemical mechanical polishing (CMP) is not needed before QD growth. The defect density in the GaAs layer of the GoVS template is estimated to be on the order of ∼108 cm−2 by plan- view transmission electron microscopy (TEM). Both TEM and x-ray diffraction suggest a three- to four-fold reduction of defects, as compared to blanket heteroepitaxy of GaAs on offcut Si wafers . Figure 1(c) shows a schematic illustration of the epitaxial layers. The micro-disk laser structure, which is composed of a 1 μm GaAs buffer, a 600 nm Al0.7Ga0.3As post region, and a 500 nm disk region, was grown in a molecular beam epitaxy (MBE) system . We have deployed a five- layer InAs/InGaAs dot-in-a-well (DWELL) structure in the disk region, where the five stacked InAs quantum dots em- bedded in In0.15Ga0.85As quantum wells are separated by 37.5 nm GaAs barriers and enclosed by outer 50 nm thick Al0.4Ga0.6As barriers. The density of the quantum dots is roughly 4.3 × 1010 cm−2. Figures 1(d) and 1(e) display high- resolution TEM images of the hetero-interface between GaAs and Si. The 4.1% lattice mismatch is accommodated by the formation of a few nanometer-thick stacking faults, mostly
trapped within the diamond-shaped pockets [Fig. 1(f )]. In Fig. 1(g), we compare room temperature photoluminescence (PL) from the as-grown laser structure on the GoVS template and a GaAs substrate at a pump power density of 4.7 kW∕cm2. The peak PL intensity from the QDs on GoVS is about 2.5 times lower than the QDs grown on GaAs, with an 18 nm blueshift in the peak wavelength. The high pump power results in the saturation of ground state emission which centers in the 1.3 μm telecommunication band and gives rise to emissions from excited states on the high energy side.
The micro-disks were fabricated using 4 μm silica beads dis- persed onto the samples as hard masks for a subsequent ion- assisted etching process. After delineation of the cylinder mesa feature, acetone in an ultrasonic bath was used to remove the remaining SiO2 microspheres. The pedestal layer was defined by subsequent immersion in a 5% HF solution, which has extreme selectivity in etching AlGaAs with high Al composition in preference to the GaAs disk area. The disk was undercut by ∼1.6 μm laterally from the outer periphery to achieve effec- tive confinement of the optical modes and avoid leakage into the substrate through evanescent wave coupling. Figures 2(a) and 2(b) present 90° and 70° tilted scanning electron micro- scope (SEM) images of one micro-disk on silicon, revealing a straight vertical etching profile and smooth sidewall surface, crucial for the quality of the resonant modes. Figure 2(c) presents a top-down view of the micro-disk, showing its circular geometry.
The fabricated devices were characterized in a micro-photo- luminescence (μPL) system at room temperature. The sample was excited by a 532 nm CW diode laser with spot size focused to approximately 4 μm in diameter. Figure 3(a) shows a rep- resentative set of spectra measured from a 4 μm diameter micro-disk on silicon with progressively higher pump power from a 532 nm CW diode laser, denoting the transition from the spontaneous emission regime to the laser oscillation regime. At a low pump intensity of 165 μW, we observe a weak cavity mode at 1308 nm accompanied by a broad background emis- sion. The sub-threshold emission was fit with bi-Lorentzian curves to extract the broad InAs QDs PL background and the narrow cavity emission, as shown in Fig. 3(b). The extracted
Fig. 1. Epi